meddic
<?php <div id="mw-page-header-links">
a person who is a participating member of an organization; "the club issues a list of members, both the actives and the retirees"
tending to become more severe or wider in scope; "active tuberculosis"
in operation; "keep hope alive"; "the tradition was still alive"; "an active tradition" (同)alive
engaged in or ready for military or naval operations; "on active duty"; "the platoon is combat-ready"; "review the fighting forces" (同)combat-ready, fighting
(used of verbs (e.g. `to run' (同)dynamic
taking part in an activity; "an active member of the club"; "he was politically active"; "the participating organizations" (同)participating
(of e.g. volcanos) capable of erupting
(of e.g. volcanos) erupting or liable to erupt; "active volcanos"
(of the sun) characterized by an increased occurrence of sunspots and flares and radio emissions
characterized by energetic activity; "an active toddler"; "active as a gazelle"; "an active man is a man of action"
disposed to take action or effectuate change; "a director who takes an active interest in corporate operations"; "an active antagonism"; "he was active in drawing attention to their grievances"
engaged in full-time work; "active duty"; "though past retirement age he is still active in his profession"
exerting influence or producing a change or effect; "an active ingredient"
expressing that the subject of the sentence has the semantic function of actor: "Hemingway favors active constructions"
full of activity or engaged in continuous activity; "an active seaport"; "an active bond market"; "an active account"
an abundant nonmetallic tetravalent element occurring in three allotropic forms: amorphous carbon and graphite and diamond; occurs in all organic compounds (同)C, atomic number 6
a copy made with carbon paper (同)carbon_copy
PrepTutorEJDIC
『活動的な』,活発な,活気のある / 『有効な』,(薬の効力などが)まだ働いている,機能している / (軍務で)現役の / 『積極的な』,実際的な / 能動態の
『炭素』(化学記号は『C』) / 〈C〉炭素棒 / 〈C〉《時に〈U〉》=carbon paper
Wikipedia preview
出典(authority):フリー百科事典『ウィキペディア(Wikipedia)』「2015/02/06 23:27:52」(JST)
wiki en
[Wiki en表示]
This article's lead section may not adequately summarize key points of its contents. Please consider expanding the lead to provide an accessible overview of all important aspects of the article. (September 2012)
Activated carbon, also called activated charcoal, activated coal, or carbo activatus, is a form of carbon processed to have small, low-volume pores that increase the surface area available for adsorption or chemical reactions.[1] Activated is sometimes substituted with active.
Due to its high degree of microporosity, just one gram of activated carbon has a surface area in excess of 500 m2, as determined by gas adsorption. An activation level sufficient for useful application may be attained solely from high surface area; however, further chemical treatment often enhances adsorption properties.
Activated carbon is usually derived from charcoal and increasingly, high-porosity biochar.
1.1 Medical uses
1.2 Adverse drug effects
1.3 Analytical chemistry applications
1.4 Environmental applications
1.5 Fuel storage
1.6 Gas purification
1.7 Chemical purification
1.8 Sound Absorption
1.9 Distilled alcoholic beverage purification
1.10 Mercury scrubbing
1.10.1 Disposal in the USA after absorbing mercury
3.1 Powdered activated carbon (R 1, PAC)
3.2 Granular activated carbon (GAC)
3.3 Extruded activated carbon (EAC)
3.4 Bead activated carbon (BAC)
3.5 Impregnated carbon
3.6 Polymer coated carbon
4.1 Iodine number
4.2 Molasses
4.3 Tannin
4.4 Methylene blue
4.5 Dechlorination
4.6 Apparent density
4.7 Hardness/abrasion number
4.8 Ash content
4.9 Carbon tetrachloride activity
4.10 Particle size distribution
5 Modification of properties and reactivity
6 Examples of adsorption
6.1 Heterogeneous catalysis
6.2 Absorption refrigeration
7 Reactivation and regeneration
7.1 Thermal reactivation
7.2 Other regeneration techniques
Activated carbon is used in gas purification, decaffeination, gold purification, metal extraction, water purification, medicine, sewage treatment, air filters in gas masks and respirators, filters in compressed air and many other applications.
One major industrial application involves use of activated carbon in the metal finishing field. It is very widely employed for purification of electroplating solutions. For example, it is a main purification technique for removing organic impurities from bright nickel plating solutions. A variety of organic chemicals are added to plating solutions for improving their deposit qualities and for enhancing properties like brightness, smoothness, ductility, etc. Due to passage of direct current and electrolytic reactions of anodic oxidation and cathodic reduction, organic additives generate unwanted breakdown products in solution. Their excessive build up can adversely affect the plating quality and physical properties of deposited metal. Activated carbon treatment removes such impurities and restores plating performance to the desired level.
Medical uses
Main article: Activated charcoal (medication)
Activated charcoal for medical use
Activated carbon is used to treat poisonings and overdoses following oral ingestion. It is not effective for a number of poisonings including: strong acids or alkali, iron, lithium, arsenic, methanol, ethanol or ethylene glycol.[2]
Adverse drug effects
Incorrect application (e.g. into the lungs) results in pulmonary aspiration which can sometimes be fatal if immediate medical treatment is not initiated.[3] The use of activated carbon is contraindicated when the ingested substance is an acid, an alkali, or a petroleum product.
Analytical chemistry applications
Activated carbon, in 50% w/w combination with celite, is used as stationary phase in low-pressure chromatographic separation of carbohydrates (mono-, di-trisaccharides) using ethanol solutions (5–50%) as mobile phase in analytical or preparative protocols.
Environmental applications
Activated carbon is usually used in water filtration systems. In this illustration, the activated carbon is in the fourth level (counted from bottom).
Carbon adsorption has numerous applications in removing pollutants from air or water streams both in the field and in industrial processes such as:
Spill cleanup
Groundwater remediation
Volatile organic compounds capture from painting, dry cleaning, gasoline dispensing operations, and other processes.
In 2007, UGent (Ghent University, Belgium) began research in water treatment after festivals.[4] A full scale activated carbon installation was built at the Dranouter music festival in 2008, with plans to utilize the technology to treat water at this festival for the next 20 years.[4]
Activated carbon is also used for the measurement of radon concentration in air.
Research is being done testing various activated carbons' ability to store natural gas and hydrogen gas. The porous material acts like a sponge for different types of gases. The gas is attracted to the carbon material via Van der Waals forces. Some carbons have been able to achieve bonding energies of 5–10 kJ per mol. The gas may then be desorbed when subjected to higher temperatures and either combusted to do work or in the case of hydrogen gas extracted for use in a hydrogen fuel cell. Gas storage in activated carbons is an appealing gas storage method because the gas can be stored in a low pressure, low mass, low volume environment that would be much more feasible than bulky on board compression tanks in vehicles. The United States Department of Energy has specified certain goals to be achieved in the area of research and development of nano-porous carbon materials. All of the goals are yet to be satisfied but numerous institutions, including the ALL-CRAFT program,[5] are continuing to conduct work in this promising field.
Gas purification
Filters with activated carbon are usually used in compressed air and gas purification to remove oil vapours, odour, and other hydrocarbons from the air. The most common designs use a 1 stage or 2 stage filtration principle in which activated carbon is embedded inside the filter media. Activated carbon is also used in spacesuit Primary Life Support Systems. Activated carbon filters are used to retain radioactive gases from a nuclear boiling water reactor turbine condenser. The air vacuumed from the condenser contains traces of radioactive gases. The large charcoal beds absorb these gases and retain them while they rapidly decay to non-radioactive solid species. The solids are trapped in the charcoal particles, while the filtered air passes through.
Chemical purification
Activated carbon is commonly used on the laboratory scale to purify solutions of organic molecules containing unwanted colored organic impurities.
Sound Absorption
Activated carbon can filter air and water. Sound energy is found within air and water and activated carbon can be used to absorb that energy. With its high degree of porosity in each activated carbon granule, sound energy has numerous areas to enter into and be converted to heat. With the energy change to heat, the process of sound absorption occurs.
Activated carbon in its granule form can be used to absorb middle and high frequency ranges provided the absorber's design lets air pass through the carbon. Activated carbon can also be used inside of diaphragmatic absorption technology to increase the rate of absorption within the diaphragmatic absorber.[6]
Distilled alcoholic beverage purification
See also: Lincoln County Process
Activated carbon filters can be used to filter vodka and whiskey of organic impurities which can affect color, taste, and odor. Passing an organically impure vodka through an activated carbon filter at the proper flow rate will result in vodka with an identical alcohol content and significantly increased organic purity, as judged by odor and taste.[citation needed]
Mercury scrubbing
Activated carbon, often impregnated with sulfur[7] or iodine, is widely used to trap mercury emissions from coal-fired power stations, medical incinerators, and from natural gas at the wellhead. This carbon is a specialty product costing more than US$4.00 per kg. However, it is often not recycled.
Disposal in the USA after absorbing mercury
The mercury-laden activated carbon presents a disposal dilemma.[8] If the activated carbon contains less than 260 ppm mercury, United States federal regulations allow it to be stabilized (for example, trapped in concrete) for landfilling.[citation needed] However, waste containing greater than 260 ppm is considered to be in the high-mercury subcategory and is banned from landfilling (Land-Ban Rule).[citation needed] This material is now accumulating in warehouses and in deep abandoned mines at an estimated rate of 1000 tons per year.[citation needed]
The problem of disposal of mercury-laden activated carbon is not unique to the United States. In the Netherlands, this mercury is largely recovered[9] and the activated carbon is disposed of by complete burning.
Activated carbon is carbon produced from carbonaceous source materials such as nutshells, coconut husk, peat, wood, coir, lignite, coal, and petroleum pitch. It can be produced by one of the following processes:
Physical reactivation: The source material is developed into activated carbons using hot gases. This is generally done by using one or a combination of the following processes:
Carbonization: Material with carbon content is pyrolyzed at temperatures in the range 600–900 °C, usually in inert atmosphere with gases like argon or nitrogen
Activation/Oxidation: Raw material or carbonized material is exposed to oxidizing atmospheres (oxygen or steam) at temperatures above 250 °C, usually in the temperature range of 600–1200 °C.
Chemical activation: Prior to carbonization, the raw material is impregnated with certain chemicals. The chemical is typically an acid, strong base, or a salt [10] (phosphoric acid, potassium hydroxide, sodium hydroxide, calcium chloride, and zinc chloride 25%). Then, the raw material is carbonized at lower temperatures (450–900 °C). It is believed that the carbonization / activation step proceeds simultaneously with the chemical activation[clarification needed]. Chemical activation is preferred over physical activation owing to the lower temperatures and shorter time needed for activating material.
Activated carbons are complex products which are difficult to classify on the basis of their behaviour, surface characteristics and other fundamental criteria. However, some broad classification is made for general purpose based on their size, preparation methods, and industrial applications.
Powdered activated carbon (R 1, PAC)
A micrograph of activated charcoal (R 1) under bright field illumination on a light microscope. Notice the fractal-like shape of the particles hinting at their enormous surface area. Each particle in this image, despite being only around 0.1 mm across, has a surface area of several square metres.[11] The entire image covers a region of approximately 1.1 by 0.7 mm, and the full resolution version is at a scale of 6.236 pixels/μm.
Normally, activated carbons (R 1) are made in particulate form as powders or fine granules less than 1.0 mm in size with an average diameter between 0.15 and 0.25 mm. Thus they present a large surface to volume ratio with a small diffusion distance[clarification needed]. Activated carbon (R 1) is defined as the activated carbon particles retained on a 50-mesh sieve (0.297 mm).
PAC material is finer material. PAC is made up of crushed or ground carbon particles, 95–100% of which will pass through a designated mesh sieve. The ASTM classifies particles passing through an 80-mesh sieve (0.177 mm) and smaller as PAC. It is not common to use PAC in a dedicated vessel, due to the high head loss that would occur. Instead, PAC is generally added directly to other process units, such as raw water intakes, rapid mix basins, clarifiers, and gravity filters.
Granular activated carbon (GAC)
A micrograph of activated charcoal (GAC) under scanning electron microscope
Granular activated carbon has a relatively larger particle size compared to powdered activated carbon and consequently, presents a smaller external surface. Diffusion of the adsorbate is thus an important factor. These carbons are suitable for absorption of gases and vapors, because they diffuse rapidly. Granulated carbons are used for water treatment, deodorization and separation of components of flow system and is also used in rapid mix basins. GAC can be either in granular or extruded form. GAC is designated by sizes such as 8×20, 20×40, or 8×30 for liquid phase applications and 4×6, 4×8 or 4×10 for vapor phase applications. A 20×40 carbon is made of particles that will pass through a U.S. Standard Mesh Size No. 20 sieve (0.84 mm) (generally specified as 85% passing) but be retained on a U.S. Standard Mesh Size No. 40 sieve (0.42 mm) (generally specified as 95% retained). AWWA (1992) B604 uses the 50-mesh sieve (0.297 mm) as the minimum GAC size. The most popular aqueous phase carbons are the 12×40 and 8×30 sizes because they have a good balance of size, surface area, and head loss characteristics.
Extruded activated carbon (EAC)
Extruded activated carbon combines powdered activated carbon with a binder, which are fused together and extruded into a cylindrical shaped activated carbon block with diameters from 0.8 to 130 mm. These are mainly used for gas phase applications because of their low pressure drop, high mechanical strength and low dust content. Also sold as CTO filter (Chlorine, Taste, Odor).
Bead activated carbon (BAC)
Bead activated carbon is made from petroleum pitch and supplied in diameters from approximately 0.35 to 0.80 mm. Similar to EAC, it is also noted for its low pressure drop, high mechanical strength and low dust content, but with a smaller grain size. Its spherical shape makes it preferred for fluidized bed applications such as water filtration.
Impregnated carbon
Porous carbons containing several types of inorganic impregnate such as iodine, silver, cations such as Al, Mn, Zn, Fe, Li, Ca have also been prepared for specific application in air pollution control especially in museums and galleries. Due to its antimicrobial and antiseptic properties, silver loaded activated carbon is used as an adsorbent for purification of domestic water. Drinking water can be obtained from natural water by treating the natural water with a mixture of activated carbon and Al(OH)3, a flocculating agent. Impregnated carbons are also used for the adsorption of Hydrogen Sulfide(H2S) and thiols. Absorption rates for H2S as high as 50% by weight have been reported.
Polymer coated carbon
This is a process by which a porous carbon can be coated with a biocompatible polymer to give a smooth and permeable coat without blocking the pores. The resulting carbon is useful for hemoperfusion. Hemoperfusion is a treatment technique in which large volumes of the patient's blood are passed over an adsorbent substance in order to remove toxic substances from the blood.
Activated carbon is also available in special forms such as cloths and fibres. The "carbon cloth" for instance is used in personnel protection for the military.
A gram of activated carbon can have a surface area in excess of 500 m2, with 1500 m2 being readily achievable.[12] Carbon aerogels, while more expensive, have even higher surface areas, and are used in special applications.
Under an electron microscope, the high surface-area structures of activated carbon are revealed. Individual particles are intensely convoluted and display various kinds of porosity; there may be many areas where flat surfaces of graphite-like material run parallel to each other, separated by only a few nanometers or so. These micropores provide superb conditions for adsorption to occur, since adsorbing material can interact with many surfaces simultaneously. Tests of adsorption behaviour are usually done with nitrogen gas at 77 K under high vacuum, but in everyday terms activated carbon is perfectly capable of producing the equivalent, by adsorption from its environment, liquid water from steam at 100 °C and a pressure of 1/10,000 of an atmosphere.
James Dewar, the scientist after whom the Dewar (vacuum flask) is named, spent much time studying activated carbon and published a paper regarding its adsorption capacity with regard to gases.[13] In this paper, he discovered that cooling the carbon to liquid nitrogen temperatures allowed it to adsorb significant quantities of numerous air gases, among others, that could then be recollected by simply allowing the carbon to warm again and that coconut based carbon was superior for the effect. He uses oxygen as an example, wherein the activated carbon would typically adsorb the atmospheric concentration (21%) under standard conditions, but release over 80% oxygen if the carbon was first cooled to low temperatures.
Physically, activated carbon binds materials by van der Waals force or London dispersion force.
Activated carbon does not bind well to certain chemicals, including alcohols, diols, strong acids and bases, metals and most inorganics, such as lithium, sodium, iron, lead, arsenic, fluorine, and boric acid.
Activated carbon adsorbs iodine very well. The iodine capacity, mg/g, (ASTM D28 Standard Method test) may be used as an indication of total surface area.
Carbon monoxide is not well adsorbed by activated carbon. This should be of particular concern to those using the material in filters for respirators, fume hoods or other gas control systems as the gas is undetectable to the human senses, toxic to metabolism and neurotoxic.
Substantial lists of the common industrial and agricultural gases adsorbed by activated carbon can be found online.[14]
Activated carbon can be used as a substrate for the application of various chemicals to improve the adsorptive capacity for some inorganic (and problematic organic) compounds such as hydrogen sulfide (H2S), ammonia (NH3), formaldehyde (HCOH), mercury (Hg) and radioactive iodine-131(131I). This property is known as chemisorption.
Iodine number
Many carbons preferentially adsorb small molecules. Iodine number is the most fundamental parameter used to characterize activated carbon performance. It is a measure of activity level (higher number indicates higher degree of activation), often reported in mg/g (typical range 500–1200 mg/g). It is a measure of the micropore content of the activated carbon (0 to 20 Å, or up to 2 nm) by adsorption of iodine from solution. It is equivalent to surface area of carbon between 900 m²/g and 1100 m²/g. It is the standard measure for liquid phase applications.
Iodine number is defined as the milligrams of iodine adsorbed by one gram of carbon when the iodine concentration in the residual filtrate is 0.02 normal. Basically, iodine number is a measure of the iodine adsorbed in the pores and, as such, is an indication of the pore volume available in the activated carbon of interest. Typically, water treatment carbons have iodine numbers ranging from 600 to 1100. Frequently, this parameter is used to determine the degree of exhaustion of a carbon in use. However, this practice should be viewed with caution as chemical interactions with the adsorbate may affect the iodine uptake giving false results. Thus, the use of iodine number as a measure of the degree of exhaustion of a carbon bed can only be recommended if it has been shown to be free of chemical interactions with adsorbates and if an experimental correlation between iodine number and the degree of exhaustion has been determined for the particular application.
Some carbons are more adept at adsorbing large molecules. Molasses number or molasses efficiency is a measure of the mesopore content of the activated carbon (greater than 20 Å, or larger than 2 nm) by adsorption of molasses from solution. A high molasses number indicates a high adsorption of big molecules (range 95–600). Caramel dp (decolorizing performance) is similar to molasses number. Molasses efficiency is reported as a percentage (range 40%–185%) and parallels molasses number (600 = 185%, 425 = 85%). The European molasses number (range 525–110) is inversely related to the North American molasses number.
Molasses Number is a measure of the degree of decolorization of a standard molasses solution that has been diluted and standardized against standardized activated carbon. Due to the size of color bodies, the molasses number represents the potential pore volume available for larger adsorbing species. As all of the pore volume may not be available for adsorption in a particular waste water application, and as some of the adsorbate may enter smaller pores, it is not a good measure of the worth of a particular activated carbon for a specific application. Frequently, this parameter is useful in evaluating a series of active carbons for their rates of adsorption. Given two active carbons with similar pore volumes for adsorption, the one having the higher molasses number will usually have larger feeder pores resulting in more efficient transfer of adsorbate into the adsorption space.
Tannins are a mixture of large and medium size molecules. Carbons with a combination of macropores and mesopores adsorb tannins. The ability of a carbon to adsorb tannins is reported in parts per million concentration (range 200 ppm–362 ppm).
Some carbons have a mesopore (20 Å to 50 Å, or 2 to 5 nm) structure which adsorbs medium size molecules, such as the dye methylene blue. Methylene blue adsorption is reported in g/100g (range 11–28 g/100g).
Dechlorination
Some carbons are evaluated based on the dechlorination half-life length, which measures the chlorine-removal efficiency of activated carbon. The dechlorination half-value length is the depth of carbon required to reduce the chlorine level of a flowing stream from 5 ppm to 3.5 ppm. A lower half-value length indicates superior performance.
Apparent density
The solid or skeletal density of activated carbons will typically range between 2.0 and 2.1 g/cm3 (125–130 lbs./cubic foot). However, a large part of an activated carbon sample will consist of air space between particles, and the actual or apparent density will therefore be lower, typically 0.4 to 0.5 g/cm3 (25–31 lbs./cubic foot).[15]
Higher density provides greater volume activity and normally indicates better-quality activated carbon.
Hardness/abrasion number
It is a measure of the activated carbon's resistance to attrition. It is an important indicator of activated carbon to maintain its physical integrity and withstand frictional forces imposed by backwashing, etc. There are large differences in the hardness of activated carbons, depending on the raw material and activity level.
Ash reduces the overall activity of activated carbon and it reduces the efficiency of reactivation. The metal oxides (Fe2O3) can leach out of activated carbon resulting in discoloration. Acid/water soluble ash content is more significant than total ash content. Soluble ash content can be very important for aquarists, as ferric oxide can promote algal growths. A carbon with a low soluble ash content should be used for marine, freshwater fish and reef tanks to avoid heavy metal poisoning and excess plant/algal growth.
Carbon tetrachloride activity
Measurement of the porosity of an activated carbon by the adsorption of saturated carbon tetrachloride vapour.
The finer the particle size of an activated carbon, the better the access to the surface area and the faster the rate of adsorption kinetics. In vapour phase systems this needs to be considered against pressure drop, which will affect energy cost. Careful consideration of particle size distribution can provide significant operating benefits.
Modification of properties and reactivity
Acid-base, oxidation-reduction and specific adsorption characteristics are strongly dependent on the composition of the surface functional groups.[16]
The surface of conventional activated carbon is reactive, capable of oxidation by atmospheric oxygen and oxygen plasma[17][18][19][20][21][22][23][24] steam,[25][26][27] and also carbon dioxide [21] and ozone.[28][29][30]
Oxidation in the liquid phase is caused by a wide range of reagents (HNO3, H2O2, KMnO4),[31][32][33]
Through the formation of a large number of basic and acidic groups on the surface of oxidized carbon to sorption and other properties can differ significantly from the unmodified forms.[16]
Activated carbon can be nitrogenated by natural products or polymers[34][35] or processing of carbon with nitrogenating reagents.[36][37][38]
Activated carbon can interact with chlorine,[39][40] bromine[41] and fluorine.[42]
Sulfonic acid functional groups can be attached to activated carbon to give "starbons" which can be used to selectively catalyse the esterification of fatty acids.[43] Formation of such activated carbons from halogenated precursors gives a more effective catalyst which is thought to be a result of remaining halogens improving stability.[44]
Some of the chemical properties of activated carbon have been attributed to presence of the surface active carbon double bond.[30][45]
The Polyani adsorption theory is a popular method for analyzing adsorption of various organic substances to their surface.
Examples of adsorption
Heterogeneous catalysis
The most commonly encountered form of chemisorption in industry, occurs when a solid catalyst interacts with a gaseous feedstock, the reactant/s. The adsorption of reactant/s to the catalyst surface creates a chemical bond, altering the electron density around the reactant molecule and allowing it to undergo reactions that would not normally be available to it.
Absorption refrigeration
Absorption refrigeration and heat pump cycles rely on the adsorption of a refrigerant gas into an adsorbent at low pressure and subsequent desorption by heating. The adsorbent acts as a "chemical compressor" driven by heat and is, from this point of view, the "pump" of the system. It consists of a solar collector, a condenser or heat-exchanger and an evaporator that is placed in a refrigerator box. The inside of the collector is lined with an adsorption bed packed with activated carbon adsorbed with methanol. The refrigerator box is insulated and filled with water. The activated carbon can adsorb a large amount of methanol vapours in ambient temperature and desorb it at a higher temperature (around 100 degrees Celsius). During the daytime, the sunshine irradiates the collector, so the collector is heated up and the methanol is desorbed from the activated carbon. In desorption, the liquid methanol adsorbed in the charcoal heats up and vaporizes. The methanol vapour condenses and is stored in the evaporator.
At night, the collector temperature decreases to the ambient temperature, and the charcoal adsorbs the methanol from the evaporator. The liquid methanol in the evaporator vaporizes and absorbs the heat from the water contained in the trays. Since adsorption is a process of releasing heat, the collector must be cooled efficiently at night. As mentioned above, the adsorption refrigeration system operates in an intermittent way to produce the refrigerating effect.
Helium gas can also be "pumped" by thermally cycling activated carbon "sorption pumps" between 4 kelvins and higher temperatures. An example of this is to provide the cooling power for the Oxford Instruments AST series dilution refrigerators. 3He vapour is pumped from the surface of the dilute phase of a mixture of liquid 4He and its isotope 3He. The 3He is adsorbed onto the surfaces of the carbon at low temperature (typically <4K), the regeneration of the pump between 20 and 40 K returns the 3He to the concentrated phase of the liquid mixture. Cooling occurs at the interface between the two liquid phases as 3He "evaporates" across the phase boundary. If more than one pump is present in the system a continuous flow of gas and hence constant cooling power can be obtained, by having one sorption pump regenerating while the other is pumping. Systems such as this allow temperatures as low as 10 mK (0.01 kelvin) to be obtained with very few moving parts.
Reactivation and regeneration
World's largest reactivation plant located in Feluy, Belgium.
Activated carbon reactivation center in Roeselare, Belgium.
The reactivation or the regeneration of activated carbons involves restoring the adsorptive capacity of saturated activated carbon by desorbing adsorbed contaminants on the activated carbon surface.
Thermal reactivation
The most common regeneration technique employed in industrial processes is thermal reactivation.[46] The thermal regeneration process generally follows three steps:[47]
Adsorbent drying at approximately 105 °C
High temperature desorption and decomposition (500–900 °C) under an inert atmosphere
Residual organic gasification by an oxidising gas (steam or carbon dioxide) at elevated temperatures (800 °C)
The heat treatment stage utilises the exothermic nature of adsorption and results in desorption, partial cracking and polymerization of the adsorbed organics. The final step aims to remove charred organic residue formed in the porous structure in the previous stage and re-expose the porous carbon structure regenerating its original surface characteristics. After treatment the adsorption column can be reused. Per adsorption-thermal regeneration cycle between 5–15 wt% of the carbon bed is burnt off resulting in a loss of adsorptive capacity.[48] Thermal regeneration is a high energy process due to the high required temperatures making it both an energetically and commercially expensive process.[47] Plants that rely on thermal regeneration of activated carbon have to be of a certain size before it is economically viable to have regeneration facilities onsite. As a result it is common for smaller waste treatment sites to ship their activated carbon cores to a specialised facility for regeneration, increasing the process' already significant carbon footprint.[49]
Other regeneration techniques
Current concerns with the high energy/cost nature of thermal regeneration of activated carbon has encouraged research into alternative regeneration methods to reduce the environmental impact of such processes. Though several of the regeneration techniques cited have remained areas of purely academic research, some alternatives to thermal regeneration systems have been employed in industry. Current alternative regeneration methods are:
Chemical and solvent regeneration[50]
Microbial regeneration[51]
Electrochemical regeneration[52]
Ultrasonic regeneration[53]
Wet air oxidation[54]
Carbon filtering
Conjugated microporous polymer
Kværner-process
Onboard refueling vapor recovery
Carbocatalysis
^ ""Properties of Activated Carbon", CPL Caron Link, accessed 2008-05-02". Retrieved 13 October 2014.
^ "Charcoal, Activated". The American Society of Health-System Pharmacists. Retrieved 23 April 2014.
^ Elliott CG, Colby TV, Kelly TM, Hicks HG (1989). "Charcoal lung. Bronchiolitis obliterans after aspiration of activated charcoal". Chest 96 (3): 672–4. doi:10.1378/chest.96.3.672. PMID 2766830.
^ a b Sustainable wastewater treatment of temporary events: the Dranouter Music Festival case study</a>. Water science and technology : a journal of the International Association on Water Pollution Research. 2008;58(8):1653–7.
^ "Alliance for Collaborative Research in Alternative Fuel Technology". All-craft.missouri.edu. Retrieved 2014-03-13.
^ Foley, Dennis (2014). "Bass Absorption - Why The Power Of Diaphragmatic Absorption Is Your Only Hope". Retrieved 2014-01-15.
^ Bourke, Marta (1989). "Activated Carbon for Mercury Removal". Retrieved 2013-08-27.
^ Tim Flannery, Here On Earth: A New Beginning, Allen Lane (2011), p. 186.
^ "''BMT-Begemann, Mercury waste treatment facilities''". Bmt-begemann.nl. Retrieved 2014-03-13.
^ J.Romanos et al. (2012). "Nanospace engineering of KOH activated carbon". Nanotechnology 23 (1): 015401. doi:10.1088/0957-4484/23/1/015401.
^ "What Is Activated Carbon?". Cabot Norit. Retrieved 24 October 2013.
^ Value Added Products from Gasification – Activated Carbon, By Shoba Jhadhav, The Combustion, Gasification and Propulsion Laboratory(CGPL)at the Indian Institute of Science(IISc)
^ The separation of the most volatile gases from air without liquefaction
^ "SentryAir". SentryAir. Retrieved 2014-03-13.
^ TIGG Corporation. Granular activated carbon selection. Published 2012-05-8, retrieved 2012-09-21.
^ a b Philippe Serp, José Luis Figueiredo, Carbon Materials for Catalysis, Wiley, – 2009, – 550 p.
^ Gómez-Serrano, V.; Piriz-Almeida, F. N.; Durán-Valle, C. J.; Pastor-Villegas, J. (1999). "Formation of oxygen structures by air activation. A study by FT-IR spectroscopy". Carbon 37 (10): 1517. doi:10.1016/S0008-6223(99)00025-1.
^ Machnikowski J., Kaczmarska H., Gerus-Piasecka I., Diez M.A., Alvarez R., Garcia R. Structural modification of coal-tar pitch fractions during mild oxidation – relevance to carbonization behavior // Carbon. – 2002. –V.40. –P.1937-1947
^ Petrov N., Budinova T., Razvigorova M., Ekinci E., Yardim F., Minkova V. Preparation and characterization of carbon adsorbents from furfural // Carbon – 2000. – V.38, №15. – P.2069-2075
^ Garcia A.B., Martinez-Alonso A., Leon C. A., Tascon J.M.D. Modification of the surface properties of an activated carbon by oxygen plasma treatment // Fuel. – 1998. –V.77, №1 – P.613-624
^ a b Saha B., Tai M.H., Streat M. Study of activated carbon after oxidation and subsequent treatment characterization // Process safety and environmental protection – 2001. – V.79, №B4. – P.211-217
^ Polovina M., Babic B., Kaluderovic B., Dekanski A. Surface characterization of oxidized activated carbon cloth // Carbon −1997. – V.35, №8. – P.1047-1052
^ Fanning P.E., Vannice M.A. A DRIFTS study of the formation of surface groups on carbon by oxidation // Carbon – 1993. – V.31, №5. – P.721-730
^ Youssef A.M., Abdelbary E.M., Samra S.E., Dowidar A.M. Surface-properties of carbons obtained from polyvinyl-chloride // Ind. J. of Chem. section a-inorganic bio-inorganic physical theoretical & analytical chemistry – 1991. – V.30, №10. – P.839-843
^ Arriagada R., Garcia R., Molina-Sabio M., Rodriguez-Reinoso F. Effect of steam activation on the porosity and chemical nature of activated carbons from Eucalyptus globulus and peach stones // Microporous Mat. – 1997. – V.8, №3–4. – P.123-130
^ Molina-Sabio M., Gonzalez M.T., Rodriguez-Reinoso F., Sepulveda-Escribano A. Effect of steam and carbon dioxide activation in the micropore size distribution of activated carbon // Carbon – 1996. – V.34, №4. – P.505-509
^ Bradley RH, Sutherland I, Sheng E Carbon surface: Area, porosity, chemistry, and energy // J. of colloid and interface science – 1996. – V. 179, №2. – P. 561-569
^ Sutherland I., Sheng E., Braley R.H., Freakley P.K. Effects of ozone oxidation on carbon black surfaces // J. Mater. Sci. – 1996. – V.31. – P.5651-5655
^ Rivera-Utrilla J; Sanchez-Polo M. The role of dispersive and electrostatic interactions in the aqueous phase adsorption of naphthalenesulphonic acids on ozone-treated activated carbons // Carbon – 2002. – V.40, №14. – P.2685-2691
^ a b Valdés, H.; Sánchez-Polo, M.; Rivera-Utrilla, J.; Zaror, C. A. (2002). "Effect of Ozone Treatment on Surface Properties of Activated Carbon". Langmuir 18 (6): 2111. doi:10.1021/la010920a.
^ Pradhan B.K., Sandle N.K. Effect of different oxidizing agent treatments on the surface properties of activated carbons // Carbon. – 1999. – V.37, №8. – P.1323-1332
^ Acedo-Ramos M., Gomez-Serrano V., Valenzuella-Calahorro C., and Lopez-Peinado A.J. Oxydation of activated carbon in liquid phase. Study by FT-IR // Spectroscopy letters. – 1993. –V26(6). – P.1117-1137
^ Gomez-Serrano V., Acedo-Ramos M., Lopez-Peinado A.J., Valenzuela-Calahorro C. Stability towards heating and outgassing of activated carbon oxidized in the liquid-phase // Thermochimica Acta. – 1991. – V.176. – P.129-140
^ Stőhr B., Boehm H.P., Schlőgl R. Enhancement of the catalytic activiti of activated carbons in oxidation reactions by termal treatment with ammonia or hydrogen cyanide and observation of a superoxide species as a possible intermediate // Carbon. – 1991. – Vol. 26, № 6. – P. 707-720
^ Biniak S., Szymański G., Siedlewski J., Światkowski A. The characterizaíion of activated carbons with oxygen and nitrogen surface groups // Carbón. – 1997. – Vol.35, № 12. – P. 1799-1810
^ Boudou J.P., Chehimi M., Broniek E., Siemieniewska T., Bimer J. Adsorption of H2S or SO2 on an activated carbon cloth modified by ammonia treatment // Carbon. – 2003. – Vol. 41, № 10. – P. 1999-2007
^ Sano H., Ogawa H. Preparation and application nitrogen containing active carbons // Osaka Kogyo Gijutsu Shirenjo. – 1975. – Vol.26, №5. – P.2084-2086
^ Radkevich, V. Z.; Senko, T. L.; Wilson, K.; Grishenko, L. M.; Zaderko, A. N.; Diyuk, V. Y. (2008). "The influence of surface functionalization of activated carbon on palladium dispersion and catalytic activity in hydrogen oxidation". Applied Catalysis A: General 335 (2): 241. doi:10.1016/j.apcata.2007.11.029.
^ Evans, M. J. B.; Halliop, E.; Liang, S.; MacDonald, J. A. F. (1998). "The effect of chlorination on surface properties of activated carbon". Carbon 36 (11): 1677. doi:10.1016/S0008-6223(98)00165-1.
^ Papirer, E. N.; Lacroix, R.; Donnet, J. B.; Nansé, G. R.; Fioux, P. (1995). "XPS study of the halogenation of carbon black—Part 2. Chlorination". Carbon 33: 63. doi:10.1016/0008-6223(94)00111-C.
^ ScienceDirect.com – Carbon – XPS Study of the halogenation of carbon black-part 1. Bromination
^ Nansé, G.; Papirer, E.; Fioux, P.; Moguet, F.; Tressaud, A. (1997). "Fluorination of carbon blacks: An X-ray photoelectron spectroscopy study: III. Fluorination of different carbon blacks with gaseous fluorine at temperatures below 100 °C influence of the morphology, structure and physico-chemical characteristics of the carbon black on the fluorine fixation". Carbon 35 (4): 515. doi:10.1016/S0008-6223(97)00003-1.
^ Aldana-Pérez, A.; Lartundo-Rojas, L.; Gómez, R.; Niño-Gómez, M. E. (2012). "Sulfonic groups anchored on mesoporous carbon Starbons-300 and its use for the esterification of oleic acid". Fuel 100: 128. doi:10.1016/j.fuel.2012.02.025.
^ Diyuk, V. E.; Zaderko, A. N.; Grishchenko, L. M.; Yatsymyrskiy, A. V.; Lisnyak, V. V. (2012). "Efficient carbon-based acid catalysts for the propan-2-ol dehydration". Catalysis Communications 27: 33. doi:10.1016/j.catcom.2012.06.018.
^ Budarin, V. L.; Clark, J. H.; Tavener, S. J.; Wilson, K. (2004). "Chemical reactions of double bonds in activated carbon: Microwave and bromination methods". Chemical Communications (23): 2736. doi:10.1039/B411222A.
^ Bagreev, A.; Rhaman, H.; Bandosz, T. J (2001). "Thermal regeneration of a spent activated carbon adsorbent previously used as hydrogen sulfide adsorbent". Carbon 39 (9): 1319–1326. doi:10.1016/S0008-6223(00)00266-9.
^ a b Sabio, E.; Gonzalez, E.; Gonzalez, J. F.; Gonzalez-Garcia, C. M.; Ramiro, A.; Ganan, J (2004). "Thermal regeneration of activated carbon saturated with p-nitrophenol". Carbon 42 (11): 2285–2293. doi:10.1016/j.carbon.2004.05.007.
^ Miguel GS, Lambert SD, Graham NJ (2001). "The regeneration of field spent granular activated carbons". Water Research 35 (11): 2740–2748. doi:10.1016/S0043-1354(00)00549-2. PMID 11456174.
^ Alvarez PM, Beltrán FJ, Gómez-Serrano V, Jaramillo J, Rodríguez EM (2004). "Comparison between thermal and ozone regenerations of spent activated carbon exhausted with phenol". Water Research 38 (8): 2155–2165. doi:10.1016/j.watres.2004.01.030. PMID 15087197.
^ Martin, R. J.; Wj, N (1997). "The repeated exhaustion and chemical regeneration of activated carbon". Water Research 21 (8): 961–965. doi:10.1016/S0043-1354(87)80014-3.
^ Aizpuru A, Malhautier L, Roux JC, Fanlo JL (2003). "Biofiltration of a mixture of volatile organic compounds on granular activated carbon". Biotechnology and Bioengineering 83 (4): 479–488. doi:10.1002/bit.10691. PMID 12800142.
^ Narbaitz RM, Karimi-Jashni A (2009). "Electrochemical regeneration of granular activated carbons loaded with phenol and natural organic matter". Environmental Technology 30 (1): 27–36. doi:10.1080/09593330802422803. PMID 19213463.
^ Lim JL, Okada M (2005). "Regeneration of granular activated carbon using ultrasound". Ultrasonic-Sono-Chemistry 12 (4): 277–285. doi:10.1016/j.ultsonch.2004.02.003. PMID 15501710.
^ Shende RV, Mahajani VV (2002). "Wet oxidative regeneration of activated carbon loaded with reactive dye". Waste Management 22 (1): 73–83. doi:10.1016/S0956-053X(01)00022-8. PMID 11942707.
"Imaging the atomic structure of activated carbon" – JOURNAL OF PHYSICS: CONDENSED MATTER
Engber, Daniel (Nov. 28, 2005). "How Does Activated Carbon Work?". Slate.
Allotropes of carbon
sp3 forms
Diamond (cubic)
Lonsdaleite (hexagonal diamond)
Fullerenes (Buckminsterfullerene, C70, Higher fullerenes, Nanotubes, Nanobuds)
Glassy carbon
sp forms
Linear acetylenic carbon
mixed sp3/sp2 forms
Amorphous carbon
Carbon nanofoam
Carbide-derived carbon
hypothetical forms
Chaoite
Cubic carbon
Metallic carbon
Aggregated diamond nanorod
History of poison
Aquatic toxicology
Entomotoxicology
Toxicogenomics
Acceptable daily intake
Fixed Dose Procedure
Lethal dose
Median lethal dose (LD50)
Toxic capacity
Toxicity Class
Cathartic
Chelation therapy
Gastric lavage
Hemoperfusion
Whole bowel irrigation
1858 Bradford sweets poisoning
2007 pet food recalls
Bhopal disaster
Minamata disease
Niigata Minamata disease
Poisoning of Alexander Litvinenko
Seveso disaster
List of poisonings
Carcinogen
Hazard symbol
List of extremely hazardous substances
Index of toxicology
Chelating agents
UpToDate Contents
全文を閲覧するには購読必要です。 To read the full text you will need to subscribe.
1. 血液透析における水質の維持 maintaining water quality for hemodialysis
2. 一酸化炭素中毒 carbon monoxide poisoning
3. 一酸化炭素拡散能 diffusing capacity for carbon monoxide
4. 早期前立腺癌の男性に対する能動的サーベイランス active surveillance for men with early prostate cancer
5. ステージIの精巣胚細胞腫瘍に対する精巣摘出術後の積極的なサーベイランス active surveillance following orchiectomy for stage i testicular germ cell tumors
English Journal
An in vitro model using the IPEC-J2 cell line for efficacy and drug interaction testing of mycotoxin detoxifying agents.
Devreese M, Pasmans F, De Backer P, Croubels S.SourceDepartment of Pharmacology, Toxicology and Biochemistry, Faculty of Veterinary Medicine, Ghent University, Salisburylaan 133, 9820 Merelbeke, Belgium. Electronic address: mathias.devreese@ugent.be.
Toxicology in vitro : an international journal published in association with BIBRA.Toxicol In Vitro.2013 Feb;27(1):157-63. doi: 10.1016/j.tiv.2012.09.020. Epub 2012 Oct 16.
An in vitro model simulating the intestinal barrier for efficacy and drug interaction testing of mycotoxin detoxifying agents was developed using Transwell® cell culture inserts. Intestinal porcine epithelial cells derived from the jejunum of piglets were exposed to DON and a mycotoxin binder (effi
Hydroquinone modified chitosan/carbon film electrode for the selective detection of ascorbic acid.
Jirimali HD, Nagarale RK, Saravanakumar D, Lee JM, Shin W.SourceDepartment of Chemistry and Interdisciplinary Program of Integrated Biotechnology, Sogang University, Seoul 121-742, Republic of Korea.
Carbohydrate polymers.Carbohydr Polym.2013 Jan 30;92(1):641-4. doi: 10.1016/j.carbpol.2012.09.024. Epub 2012 Sep 16.
A redox active polymer, hydroquinone modified chitosan (Q-chitosan) was synthesized and characterized by IR and (1)H NMR spectroscopy. The nanocomposite of Q-chitosan with carbon was prepared and used to construct a stable conductive film on the electrode surface. The SEM studies confirms that the Q
Japanese Journal
Variations in fraction of absorbed photosynthetically active radiation and comparisons with MODIS data in burned black spruce forests of interior Alaska
Iwata Hiroki,Ueyama Masahito,Iwama Chie,Harazono Yoshinobu
Polar science 7(2), 113-124, 2013-06-00
… Absorption of photosynthetically active radiation (PAR) by vegetation was observed in two burned black spruce forests, one and seven years after wildfire, in interior Alaska along with several vegetation properties. … The current regional estimation of photosynthesis in boreal region based on the light-use efficiency approach and MODIS FPAR is probably overestimated, and an accurate distribution of FPAR is desired for clarifying the regional carbon exchange in boreal forests. …
NAID 110009579492
Spatial distribution of greenhouse gas concentrations in arid and semi-arid regions : A case study in East Asia
Guo M,Wang X.-F.,Li J,Yi K.-P.,Zhong G.-S.,Wang H.-M.,Tani H.
Journal of Arid Environments 91, 119-128, 2013-04-00
… Land degradation and global warming are currently highly active research topics. … Researches have verified that carbon dioxide (CO2) and methane (CH4) are major greenhouse gases (GHG) in the atmosphere and are directly affected by human activity. …
The Australian carbon pricing experience : are there any lessons for Japan?
Dabner Justin
アメリカ太平洋研究 13, 63-85, 2013-03-00
… At the forefront of this policy was to be an additional (carbon) tax on fossil fuels, strategies to promote renewable energy (in particular a feed-in tariff) and an emissions trading scheme. … Meanwhile on July 1, 2012 the Australian Government introduced a hybrid carbon tax/emissions trading scheme putting it at the cutting edge of climate change response using fiscal measures. …
Activated Carbon | Sigma-Aldrich
III. ACTIVATED CARBON What is activated carbon? Activated carbon is an internally porous microcrystalline, non-graphitic form of carbon. 1 The activation of carbons involves the exposure of carbon to an atmosphere of CO 2, CO, O 2, H ...
Adsorption / Active Carbon - Water Treatment and Purification ...
Activated carbon adsorption Adsorption is a process where a solid is used for removing a soluble substance from the water. In this process active carbon is the solid. Activated carbon is produced specifically so as to achieve a very ...
★リンクテーブル★
リンク元 「活性炭」
関連記事 「active」「carbon」
[★]
activated charcoal、active carbon
炭化水素化合物を焼成して調製した炭素末
炭化水素の網目構造に物質を吸着できる ← 炭化水素という物性からしてイオン性、大分子(蛋白と結合した
物質)、水溶性の物質は吸着しづらい、と思われる。
活性炭の吸着に関与する要素
くり返し投与が有効なのは脂溶性、非イオン性、分布容量 Vdが小さい、蛋白結合率が低い
腸管循環する物質、腸溶剤、徐放剤
吸着できる物質
SQ.480
単独投与 :アスピリン、アセトアミノフェン、バルビツレート、フェニトイン、テオフィリン、三環系抗うつ薬、四環系抗うつ薬
くり返し投与:フェノバルビタール、フェノチアジン、オピオイド、ジギトキシン、カルシウム拮抗薬、抗コリン薬
吸着できない物質
重金属
ヒ素 arsenic、鉛、水銀、鉄、亜鉛、カドミウム
イオン化分子
リチウムイオン、ナトリウムイオン、カルシウムイオン、カリウムイオン、マグネシウムイオン、フッ素イオン、ホウ素イオン
腐食性物質
酸、アルカリ
炭化水素
アルカン、アルケン、ハロゲン化アルキル、芳香族炭化水素、アルコール、アセトン、エタノール、エチレングリコール、イソプロパノール、メタノール、
1. [charged] Decontamination of poisoned adults - uptodate [1]
2. 活性炭 - wiki ja
http://ja.wikipedia.org/wiki/%E6%B4%BB%E6%80%A7%E7%82%AD
活動性の、活動期の、活動的な、行動的な、積極的な、活発な、能動的な、有効な、アクティブな
active stage、actively、activity、aggressive、behaviorally、brisk、briskly、effective、efficacious、offensive、positive、positively、valid、vigorous、vigorously
炭素、カーボン
C、carbonic
「https://meddic.jp/index.php?title=active_carbon&oldid=219570」から取得